University of Windsor University of Windsor

### Scholarship at UWindsor

### Scholarship at UWindsor

Electronic Theses and Dissertations Theses, Dissertations, and Major Papers

2011

### Development of a shear test to determine the cyclic behaviour of

### Development of a shear test to determine the cyclic behaviour of

### sheet materials

### sheet materials

Md. Samsul Sarker

University of Windsor

Follow this and additional works at: https://scholar.uwindsor.ca/etd

Recommended Citation Recommended Citation

Sarker, Md. Samsul, "Development of a shear test to determine the cyclic behaviour of sheet materials" (2011). Electronic Theses and Dissertations. 208.

https://scholar.uwindsor.ca/etd/208

This online database contains the full-text of PhD dissertations and Masters’ theses of University of Windsor students from 1954 forward. These documents are made available for personal study and research purposes only, in accordance with the Canadian Copyright Act and the Creative Commons license—CC BY-NC-ND (Attribution, Non-Commercial, No Derivative Works). Under this license, works must always be attributed to the copyright holder (original author), cannot be used for any commercial purposes, and may not be altered. Any other use would require the permission of the copyright holder. Students may inquire about withdrawing their dissertation and/or thesis from this database. For additional inquiries, please contact the repository administrator via email

**DEVELOPMENT OF A SHEAR TEST TO DETERMINE THE **

**CYCLIC BEHAVIOUR OF SHEET MATERIALS **

**by **

**Md. Samsul Alam Sarker **

A Thesis

Submitted to the Faculty of Graduate Studies

Through the Department of Mechanical, Automotive and Materials Engineering in Partial Fulfillment of the Requirements for the Degree of Master of Applied Science at the University of

Windsor

Windsor, Ontario, Canada 2011

**DEVELOPMENT OF A SHEAR TEST TO DETERMINE THE **

**CYCLIC BEHAVIOUR OF SHEET MATERIALS **

by

Md. Samsul Alam Sarker

APPROVED BY:

**Dr. S. Das, **Outside Program Reader
Department of Civil & Environmental Engineering

**Dr. J. Johrendt, **Department Reader

Department of Mechanical, Automotive and Materials Engineering

**Dr. D. Pusca, **Co**-**Advisor

Department of Mechanical, Automotive and Materials Engineering

**Dr. D. E. Green, **Advisor

Department of Mechanical, Automotive and Materials Engineering

**Dr. Biao Zhou, **Chair of Defence

Department of Mechanical, Automotive and Materials Engineering

iii

**AUTHOR’S DECLARATION OF ORIGINALITY **

I hereby certify that I am the sole author of this thesis and no part of this thesis has been

published or submitted for publication.

I certify that, to the best of my knowledge, my thesis does not infringe upon anyone’s

copyright nor violate any proprietary rights, and that any ideas, techniques, quotations, or any

other material from the work of other people included in my thesis, published or otherwise, are

fully acknowledged in accordance with the standard referencing practices. Furthermore, to the

extent that I have included copyrighted material that surpasses the bounds of fair dealing within

the meaning of the Canada Copyright Act. I certify that I have obtained a written permission

from the copyright owner(s) to include such material(s) in my thesis.

I declare that this is a true copy of my thesis, including any final revisions, as approved

by my thesis committee and the Graduate Studies office, and this thesis has not been submitted

iv

**ABSTRACT **

In many industrial stamping operations, the sheet material is subject to a series of loading

and reverse loading cycles. In order to accurately predict the outcome of such forming processes,

numerical simulation models rely on advanced constitutive models to rigorously reproduce the

cyclic work hardening behaviour of the sheet material.

The objective of this research was to develop a testing facility that is capable of

generating the experimental stress-strain data of sheet materials when they are subjected to cyclic

shearing loads. A suitable specimen geometry and a corresponding loading fixture were designed

and fabricated.

Cyclic shear tests were successfully carried out on four different grades of automotive

sheet steel using this new testing fixture mounted in a universal testing machine. The

experimental data thus generated can be used to determine the material parameters in advanced

constitutive models, in order to virtually simulate metal forming operations and the subsequent

v

**DEDICATION **

*To my parents, my wife Ferdoush Jahan, my daughters Raika Alam and Aniba Alam, for their *

vi

**ACKNOWLEDGEMENTS **

I would like to express my sincere gratitude and profound appreciation to my advisor, Dr.

D.E. Green, for his patience, invaluable supervision, guidance, continuing encouragement,

intellectual discussions, thoughtful insights, and so generously taking his time to discuss all

aspects of this research, and shared expertise in sheet metal forming throughout my graduate

studies and research. His assistance over the course of my research has been invaluable and

immeasurable; without his guidance this project would have been impossible.

I appreciate Dr. D. Pusca sharing her ideas to optimize the fixture model, apply GD&T to

parts and assembly drawings, and for mentoring me during this research. My sincere thanks to

committee member Dr. J. Johrendt for her support, valuable comments, and suggestions to

improve the model. Dr. S. Das is also acknowledged for serving on my thesis committee and

making suggestions to improve this thesis.

I would also like to thank the laboratory technologist Mr. Andy Jenner who built the

cyclic shear test fixture and specimens promptly and his assistance during testing is appreciated.

Mr. Albrecht Conle is greatly appreciated for his assistance, interactive and fruitful discussions

during the experiments. I acknowledge the work of Dr. Thuillier at the Université de

Bretagne-Sud, France, who provided experimental shear test data.

My thanks also to my fellow researcher Mr. Amir for his help and shared expertise

conducting experimental tests, and other colleagues in the CRC lab. They are greatly

appreciated for their interactive and fruitful discussions in sheet metal forming research during

this period of study. Finally, but not least, I would like to express my sincere gratitude to my

parents for encouraging me, and my wife and children for being with me throughout the long

vii

**TABLE OF CONTENTS **

AUTHOR'S DECLARATION OF ORIGINALITY ... iii

ABSTRACT ... iv

DEDICATION ...v

ACKNOWLEDGEMENTS ... vi

LIST OF FIGURES AND TABLES...x

LIST OF ABBREVIATIONS ...xv

LIST OF SYMBOLS ... xvii

1. **INTRODUCTION**...1

2. **LITERATURE REVIEW** ...6

2.1 SPRINGBACK IN STAMPED PARTS ...6

2.2 EXPERIMENTAL SPRINGBACK STUDIES AND SIMULATIVE TESTS ...9

2.3 PREDICTION OF SPRINGBACK ...15

2.3.1 Plasticity and Anisotropic Yield Functions ...15

Hill’s Yield Criteria ...16

Barlat’s Yield Criterion ...16

2.3.2 Hardening Laws ...16

Isotropic Hardening ...17

Kinematic Hardening ...18

Non Linear Kinematic Hardening ...20

Mixed Hardening ...21

Multi-surface Hardening Models ...23

2.3.3 Numerical Simulation of Springback...25

2.3.4 Optimization of Springback Predictions ...29

2.4 EXPERIMENTAL CHARACTERIZATION OF THE CYCLIC BEHAVIOUR OF METAL SHEETS ...31

2.4.1 Tension-Compression Tests ...32

viii

2.4.3 Cyclic Shear Tests...36

2.4.4 Advantages of Cyclic Shear Tests ...44

3. **DESIGN OF THE CYCLIC SHEAR TEST FIXTURE AND SPECIMEN** ...47

3.1 DESIGN METHODOLOGY ...47

3.2 DESIGN OF A CYCLIC SHEAR TEST FIXTURE ...48

3.2.1 Design of the Cyclic Shear Test Fixture ...49

Fixed Upper Part ...51

Movable Lower Part ...52

Holding Blocks ...53

Socket Head Cap Screws ...54

3.2.2 Optimization of the Cyclic Shear Test Fixture Design ...54

3.2.3 Deformation of the Test Fixture ...55

3.3 DESIGN OF A CYCLIC SHEAR TEST SPECIMEN ...57

3.3.1 Design of the Cyclic Shear Test Specimen ...58

3.3.2 Numerical Simulation of the Cyclic Shear Tests ...60

3.3.3 Optimization of the Cyclic Shear Test Specimen Design ...65

4. **EXPERIMENTAL PROCEDURES** ...71

4.1 DESCRIPTION OF SHEET MATERIALS ...71

High Strength Low Alloy (HSLA) Steels ...71

Dual Phase (DP) Steels ...72

Transformation Induced Plasticity (TRIP) Steels ...73

4.2 SPECIMEN PREPARATION ...74

4.2.1 Preparation of Tensile Test Specimens ...75

4.2.2 Cyclic Shear Test Specimen Preparation ...76

4.3 TESTING PROCEDURES ...77

4.3.1 Tensile Test Procedures ...78

4.3.2 Cyclic Shear Test Procedures ...79

4.4 SYSTEM CALIBRATION AND STRAIN MEASUREMENTS ...83

4.4.1 System Calibration ...83

4.4.2 Strain Measurements ...86

ix

5. **RESULTS AND DISCUSSIONS** ...89

5.1 EXPERIMENTAL RESULTS OF TENSILE TESTS ...89

5.1.1 DP600 Tensile Test ...90

5.1.2 DP980 Tensile Test ...91

5.1.3 TRIP780 Tensile Test ...92

5.1.4 HSLA Tensile Test ...93

5.2 EXPERIMENTAL AND SIMULATION RESULTS OF CYCLIC SHEAR TESTS ...95

5.2.1 DP600 Cyclic Shear Test ...96

5.2.2 DP980 Cyclic Shear Test ...102

5.2.3 TRIP780 Cyclic Shear Test ...107

5.2.4 HSLA Cyclic Shear Test ...111

**6. CONCLUSIONS** ...116

APPENDIX A. CYCLIC SHEAR TEST FIXTURE COMPONENTS AND ASSEMBLY DRAWINGS WITH BILL OF MATERIALS ...119

REFERENCES ...126

x

**LIST OF FIGURES **

Figure 2.1 Springback simulation of sheet metal cup in stamping ...7

Figure 2.2 Different types of springback (a) wall opening (b) wall curl (c) bow ...8

Figure 2.3 Sidewall curl in a drawn channel section ...8

Figure 2.4 Geometrical model of air bending of sheet metal ...9

Figure 2.5 Bending under tension in a typical stamping (drawing) operation ...10

Figure 2.6 Schematic of Sanchez’ three pin roller set-up for cyclic bending of sheet metal...11

Figure 2.7 Schematic of the draw-bend test, R is the roller radius,Fb is the back force, and Δθ is the springback angle ...13

Figure 2.8 Time-dependent springback in (a) DP600 (b) DP980 (c) TRIP780 strips subject to bending under tension.R/t is the roller radius to sheet thickness ratio,Fb is the back force, and δθ is the time-dependent springback angle ...13

Figure 2.9 Isotropic hardening of the yield surface with plastic deformation, and the corresponding uniaxial stress-strain curve ...18

Figure 2.10 Kinematic hardening showing (a) the transitions, | | of the yielding surface with plastic strain, and (b) the resulting stress-strain curve with shifted yield stress in compression-the Bauschinger effect ...19

Figure 2.11 Comparison of the experimental cyclic stress-strain data for DP600 sheet steel and that predicted with the NKH model ...20

Figure 2.12 Schematic illustrations of combined kinematic and isotropic hardening ...22

Figure 2.13 Schematic illustration of Yoshida-Uemori two-surface model ...24

Figure 2.14 Schematic illustration of the stress-strain behaviour of certain materials ...25

Figure 2.15 Effect of hardening model on the simulated profile of DP 600 channel section (a)at 25% (left) and (b)75% (right) drawbead penetration ...29

Figure 2.16 Schematic of double wedges uniaxial tension-compression test device ...33

Figure 2.17 Schematic of the cyclic tension-compression device developed by Boger et al. ...34

xi

Figure 2.19 Symmetrical shear test specimen geometry used by An. et al., in which L and W

are the dimensions of the gauge area; the white areas are the shear zones and the

grey areas are the clamping zones. ...39

Figure 2.20 Photograph of the simple shear device developed by Thuillier and Manach with a

close-up of the grip system ...41

Figure 2.21 Simple shear test specimen developed by Zang et al., showing the homogeneity of

the strain distribution along three sections of the gauge region (S0, S1, S2) parallel to

the shear direction, for = 0.3 and 0.6, average 1 indicates the entire gauge surface

and average 2 indicates the reduced area in the specimen center, and X denotes the

sample length ...42

Figure 2.22 Shear test facility developed by Meyer et al., showing (a) the jig and specimen (b)

the strain field in the shear zones measured with the ARAMIS system ...43

Figure 3.1 Flow diagram of the design processes for a cyclic shear test facility ...48

Figure 3.2 Photograph of(a)the INSTRON 8562 universal testing machine, (b) a CAD model

of the cyclic shear test fixture, and (c) the details of holding blocks and bolts (d) the

sheet specimen positioned in the testing fixture ...50

Figure 3.3 (a)CAD model of fixed upper part of cyclic shear fixture (b) photograph of fixed

upper part of cyclic shear test fixture ...51

Figure 3.4 (a)CAD model of movable lower part (b) photograph of movable lower part of

cyclic shear test fixture ...52

Figure 3.5 (a)CAD model of holding block (b)photograph of holding blocks of cyclic shear

test fixture with inserted circular knurled blocks ...53

Figure 3.6 (a) CAD model and, (b) photograph of a socket head cap screw ...54

Figure 3.7 Maximum deflection of the fixed upper part of the cyclic shear test fixture (a)

during tension and (b) during compression ...57

Figure 3.8 ASTM B831 shear test specimen for sheet materials ...58

Figure 3.9 (a)CAD model and (b) photograph of the proposed sheet specimen used with the

cyclic shear test fixture ...60

Figure 3.10 Comparison of the predicted stress distribution along the length of the gauge area of

xii

Figure 3.11 Comparison of the predicted strain distribution along the length of the gauge area of

the shear specimen for different mesh sizes ...63

Figure 3.12 Finite element mesh of a half-model of the shear specimen ...64

Figure 3.13 Comparison of the shear strain distribution in the gauge area of the sheet specimen for different numbers of bolt holes ...68

Figure 3.14 Drawing of the optimized cyclic shear test specimen ...70

Figure 3.15 Photograph of inserted knurled blocks on the surfaces of (a) the upper and lower fixtures, and (b) the holding blocks of the cyclic shear test fixture ...70

Figure 4.1 Stress-strain behaviour of different types of DP steels ...73

Figure 4.2 Comparison of the typical stress-strain curves of HSLA, DP and TRIP steels ...74

Figure 4.3 ASTM standards E8, geometry for tensile test specimens ...75

Figure 4.4 Painted tensile test specimens for different grade of sheets with black speckles pattern ...76

Figure 4.5 Photograph of the cyclic shear test specimens (a) without paint (b) painted with a high contrast stochastic pattern ...77

Figure 4.6 Photograph of (a) a clamped tensile specimen ready for testing, (b) the ARAMIS system with stereo cameras focussed on tensile specimen ...79

Figure 4.7 Cyclic shear test (a) experimental test set up with ARAMIS system (b) fixture set up ...80

Figure 4.8 Cyclic shear test (a) specimen set up between fixed upper and lower movable fixture (b) specimen and two shearing gauge zones of the specimen...81

Figure 4.9 ARAMIS 3D sensor unit to measure the volume of calibration panel ...84

Figure 4.10 Calibration panels for (a) 65 mm x 52 mm x 52 mm volume (b) 35 mm x 28 mm x 28 mm ...85

Figure 4.11 Digital images of a random speckle pattern: undeformed pattern as seen from (a) the left and (b) right cameras; deformed pattern as seen from (c) the left and (d) right cameras ...86

Figure 4.12 Photograph of the ARAMIS digital image analysis software showing the strain distribution in the gauge area of a shear specimen ...87

Figure 5.1 Stress-strain behaviour of DP600 sheet steel in tensile test ...91

xiii

Figure 5.3 Stress-strain behaviour of TRIP780 sheet steel in tensile test ...93

Figure 5.4 Stress-strain behaviour of HSLA sheet steel in tensile test ...94

Figure 5.5 True stress-strain curves for different sheet materials in tensile test ...94

Figure 5.6 (a) von Mises effective stress (in GPa) and (b) effective plastic strain predicted in

the gauge region of the DP600 shear specimen after a 2 mm displacement ...97

Figure 5.7 Section A-A in the centre of the gauge area of the shear specimen ...98

Figure 5.8 Predicted shear stresses and shear strains distributions along the gauge length of the

DP600 shear specimen ...99

Figure 5.9 Experimental load-displacement curves obtained by cyclic shear for DP600 steel100

Figure 5.10 Experimental shear stress-shear strain curves for DP600 steel ...100

Figure 5.11 (a) three different sections on the gauge region (b) comparison of the gauge sections

strain distributions obtained from the ARAMIS system for DP600 sheet steel ...101

Figure 5.12 ARAMIS images of the shear strain in the gauge of DP600 specimen after (a)

forward loading and (b) reverse loading ...102

Figure 5.13 Shear strain distributions measured with the ARAMIS system along the centre of

the gauge of the DP600 shear specimen after forward and reverse loading ...102

Figure 5.14 (a) von Mises effective stress (in GPa) and (b) effective plastic strain predicted in

the gauge region of DP980 shear specimen after a 2 mm displacement ...103

Figure 5.15 Predicted shear stresses and shear strains distributions along the gauge length of the

DP980 shear specimen ...104

Figure 5.16 Experimental load-displacement curves obtained by cyclic shear for DP980 steel105

Figure 5.17 Experimental shear stresses - shears strain curves for DP980 steel ...105

Figure 5.18 ARAMIS images of the shear strain in the gauge of DP980 shear specimen after (a)

forward loading and (b) reverse loading ...106

Figure 5.19 Shear strain distributions measured with the ARAMIS system along the centre of

the gauge of the DP980 shear specimen after forward and reverse loading ...106

Figure 5.20 (a) von Mises effective stress (in GPa) and (b) effective plastic strain predicted in

the gauge region of the TRIP780 shear specimen after a 2 mm displacement ...107

Figure 5.21 Predicted shear stresses and shear strains distributions along the gauge length of the

xiv

Figure 5.22 Experimental load-displacement curves obtained by cyclic shear for TRIP780

steel ...109

Figure 5.23 Experimental shear stresses - shear strains curves for TRIP780 steel ...109

Figure 5.24 ARAMIS images of shear strain distribution of TRIP780 sheet steel (a) forward

cyclic loading (b) reverse cyclic loading ...110

Figure 5.25 Shear strain distributions at the centre of the gauge section of TRIP780 steel sheet

during the cyclic loading and unloading condition obtained from ARAMIS system110

Figure 5.26 (a) von Mises effective stress (in GPa) and (b) effective plastic strain predicted in

the gauge region of the HSLA shear specimen after a 2 mm displacement ...111

Figure 5.27 Predicted shear stresses and shear strains distributions along the gauge length of the

HSLA shear specimen ...112

Figure 5.28 Experimental load-displacement curves obtained by cyclic shear for HSLA steel 113

Figure 5.29 Experimental shear stresses - shear strains curves for HSLA steel ...113

Figure 5.30 ARAMIS images of shear strain in the gauge of HSLA specimen after (a) forward

loading and (b) reverse loading ...114

Figure 5.31 Shear strain distributions measured with the ARAMIS system along the centre of

the gauge of the HSLA shear specimen after forward and reverse loading ...114

**LIST OF TABLES **

Table 3.1 Comparison of the execution times for different mesh densities ...65

Table 3.2 Comparison of the uniformity factor with respect to the number of bolt holes ...69

xv

**LIST OF ABBREVIATIONS **

AHSS Advanced High Strength Steels

AISI American Iron and Steel Institute

AKDQ Aluminum Killed Draw Quality

ANN-EA Artificial Neural Network Evolutionary Algorithm

ASTM American Society for Testing and Materials

BNC Bayonet Neill–Concelman

BPNN Back Propagation Neural Network

CAD Computer Aided Design

DAP Data Acquisition Processor

DAT Data Acquisition Tool

DIC Digital Image Correlation

DOE Design of Experiments

DP Duel Phase

DQSK Draw Quality Semi-Killed

EA Evolutionary Algorithm

EDM Electrical Discharge Machine

FE Finite Element

FEA Finite Element Analysis

FEM Finite Element Method

GA Genetic Algorithm

GA-BP Genetic Algorithm Back Propagation

GB Gigabyte

HSLA High Strength Low Alloy

HSS High Strength Steel

Hz Hertz

IH Isotropic Hardening

KN Kilo Newton

xvi

MPa Mega Pascal

NAFR Non Associate Flow Rule

NKH Non Linear Kinematic Hardening

PB Pre-stretching and Bending

RAM Random Access Memory

RD Rolling Direction

RIK Rotational Isotropic Kinematic

RS Random Search

SB Simultaneous Stretching and Bending

SD Shearing Direction

SSC Shear Tensile Stress Condition

TD Transverse Direction

TRIP Transformed Induced Plasticity

TSC Tensile Stress Condition

UTS Ultimate Tensile Strength

WS Without Stretching

xvii

**LIST OF SYMBOLS **

**Symbol ** **Description **

𝑓 Function

Effective stress (or flow stress)

_{ } Engineering stress

True stress

𝑦 Yield stress

𝑦0 Initial Yield stress

Engineering strain

_{ } True strain
Plastic strain

̅ Effective strain

𝑝 Accumulated effective plastic strain

(𝑝) Isotropic hardening function

τ, Shear stress

γ Shear strain

α-Fe Ferrite

γ-Fe Austenite

Instantaneous tensile load

Initial area

Dp Rate of plastic deformation

L0 Initial Length

Li Instantaneous Length

Natural logarithm

K Strength index of material

l Length of sheared area

Strain hardening exponent

xviii

Unit vector direction of kinematic motion

r Slot radius

w Width of sheared area

t Thickness of sheet metal

B Initial size

F Force

H Height of calibrated volume

L Length of calibrated volume

W Width of calibrated volume

R Bending radius

Ri Isotropic hardening component

S Cauchy stress deviator

Y Radius of yield surface in the deviatoric space

c Tool gap in bending

e Punch displacement in bending

w Die opening in bending

α Springback angle

αb Back stress deviator/tensor

Relative kinematic motion of the yield surface

β Center of the bounding surface

θ Bending angle

∅ Diameter

N-m Newton-meter

∆ρ Springback quantity of bending radius

∆β Springback quantity of bending angle

∆θ Changes in springback angle

δθ Time dependent springback angle

1

**1.**

**INTRODUCTION **

Sheet metal forming processes are commonly used to produce a multitude of parts for the

automotive, aerospace, appliance and farm equipment industries. The manufacture of sheet metal

components often requires one or more stamping operations in which the sheet material is

stretched, drawn and bent between two mating dies to give it the desired shape. Stamping has

actually been one of the most cost-effective ways of mass producing parts, especially for

automotive components.

In an age where fuel consumption and weight reduction have become significant

preoccupations, the automotive industry is driven to manufacture the body and structure of

passenger vehicles using either high strength steel, aluminum or magnesium sheets. In view of

the higher cost of magnesium and aluminum, however, the trend has been to use increasing

proportions of high strength steel so that body components can be produced with thinner gauges

without compromising the structural integrity (i.e. the torsional and bending stiffness) and the

crash resistance of the vehicle. In particular, advanced high strength steels (AHSS) such as dual

phase (DP) and transformed induced plasticity (TRIP) steels have now become common

automotive sheet materials, and the trend continues to be for automotive body panels and

structures to be made from steel grades that have increasing tensile strength.

The main challenges of producing sheet metal parts are, first of all, to satisfy the design

specifications in terms of the geometric dimensions and tolerances of the part, and secondly, to

avoid any defects such as excessive thinning, splits, wrinkles, surface damage and inconsistent or

uncontrolled springback. Indeed, after a part has been stamped and then removed from the dies,

2

stresses reach a state of equilibrium. The recovery of elastic deformations is an inevitable

characteristic of metallic materials that can lead to significant changes in the shape of a part. For

instance, bent shapes will tend to unbend, drawn channels will tend to exhibit sidewall curl and

open parts will tend to twist.

Springback is actually a complex phenomenon: the nature and amount of deviation from the

intended part geometry depends on the mechanical properties of the sheet material, on the level

of stresses and strains that are attained in the part at the end of the forming process, and on the

constraints that come from the shape of the part itself. Therefore, as stamped automotive parts

are made from increasingly higher strength sheet materials, the magnitude and complexity of

springback also increases. It is not surprising therefore that the single most costly challenge for

suppliers of automotive stamped parts is to control the springback.

Traditionally, springback has been minimized by stamping prototype parts and then

reworking the dies, and successively repeating this process by trial and error until the parts fit

properly in a checking fixture. However, this way of building dies can be very costly and

time-consuming, even when it is carried out by experienced tool & die makers, and may not always

lead to a well-controlled manufacturing process. Furthermore, building a production die that is

designed with incorrect springback compensation can cause significant difficulties in

downstream operations such as poor fit-up in a welded subassembly. In some cases, tooling

revisions may be required which could delay the start of production. Therefore the prediction of

springback, especially in parts made from AHSS, is of critical importance to suppliers of

automotive stampings.

The competition in the automotive industry is such that stamping dies must be designed and

3

specified by the product designer. This signifies that springback must be known and accounted

for when the dies are designed. The most efficient way for this to be done is to use

state-of-the-art numerical simulation to predict the outcome of a stamping operation. Indeed, commercial

finite element analysis (FEA) software is routinely used to dynamically simulate the stamping

process as well as predict the springback [1] after stamping for many complex automotive parts.

Once springback has been predicted for a virtual model of the part, the shape of the die can be

compensated to eliminate or minimized springback before the dies are built.

The finite element method is widely used in the industry to predict the springback of stamped

parts [1], and consists of building a virtual model of the entire stamping process with all the

tooling surfaces that interact with the sheet metal. The blank and the dies are discretized into a

large number of elements, mechanical properties are assigned to each component and the

kinematics and boundary conditions of the stamping process are virtually reproduced. During the

numerical simulation the die surfaces gradually close into their mating position by a series of

small incremental steps, and as a result of the constraints and forces applied to the blank it

progressively deforms into the desired shape. During each increment, the equations of motion are

solved at each integration point in each element of the blank and the strains and stresses are

computed. After the forming process is simulated, springback is also predicted by virtually

opening the dies and allowing the formed part to elastically unload to its equilibrium position.

The accuracy of the numerical analysis depends on a large number of factors, but in

particular on the constitutive model that is selected to describe the behaviour of the sheet

material. Much research has been devoted to developing constitutive models that are capable of

reproducing the behaviour of sheet materials, and today, various advanced constitutive models

4

springback of AHSS sheets. However, a specific series of material characterization tests must be

carried out for a given sheet material in order to determine the parameters in the constitutive

model that will describe the actual behaviour of this sheet. As constitutive models become more

advanced, they generally have more parameters that need to be determined, which means more

sophisticated characterization tests are required.

During many stamping or drawing operations the sheet metal is subjected to successive

bending and unbending during the forming process, such as when the blank is formed over a

punch or die radius. When a blank is drawn over a die radius one side of the sheet is deformed in

tension while the other side is in compression, and a gradient of deformation develops through

the thickness of the sheet. But once the sheet exits the curved portion of the tooling it straightens

out again, and the side that was in tension becomes loaded in compression, and vice versa for the

opposite side of the sheet. When sheet metal is formed through a drawbead the material

experiences a series of bending-unbending cycles. Forming operations that make use of

drawbeads to control the flow of metal are quite common and lead to cyclic loading and

unloading in specific areas of the part. It is essential therefore, that the constitutive model in the

FEA be able to accurately simulate the actual behaviour of the sheet material when it is

cyclically deformed, because unless the strains and stresses are accurately predicted in the virtual

forming process the strains and stresses (and the part shape) will obviously not be accurately

predicted after springback.

The main objective of this research is to design and build a testing apparatus that will enable

us to experimentally determine the cyclic stress-strain behaviour of sheet materials so that finite

element (FE) analysts seeking to predict the springback of stamped parts can determine the

5

The development of a test to cyclically deform sheet metal specimens involves several steps:

Selecting the type of deformation to impose on the specimen (e.g.

tension/compression, bending/unbending, simple shear etc.).

Designing and optimizing the specimen geometry with a gauge area in which stresses

and strains are uniformly distributed and can easily be measured during a test.

Designing and building a rigid fixture that can be mounted in a testing apparatus and

that can impose the desired type of cyclic loading onto the specimen.

Once the prototype fixture is built and sheet specimens are fabricated, it will be necessary to

carry out tests to verify that the specimens, fixture and testing actually provide the desired

experimental stress-strain data.

This thesis divides into six chapters. Chapter 2 provides a review of springback and the

current constitutive models used to simulate the deformation of anisotropic sheet materials.

Moreover, a literature review of various testing facilities that have been used to experimentally

determine the cyclic behaviour of sheet materials is also provided. Chapter 3 presents a

description of the methodology that was followed to design both the test fixture and the

geometry of the sheet specimen. Chapter 4 presents the experimental work that was done to

verify the effectiveness of the test, including the different sheet materials that were tested, the

testing procedures, the strain measurements and the details of data analysis. Chapter 5 provides

the experimental stress-strain response of the sheet materials that were tested. Finally, Chapter 6

presents the observations made throughout this experimental work as well as some conclusions

6

**2. LITERATURE REVIEW **

Before one can design a testing apparatus to experimentally determine the cyclic

stress-strain behaviour of AHSS sheets it is necessary to first consider the work that other researchers

have done to characterize and model the cyclic behaviour of sheet materials. This chapter

provides an overview of the literature relevant to this study and divides into four main sections.

The first section briefly describes the types of springback that can develop in industrial sheet

metal components. The next section provides an overview of some simulative tests that have

been developed to experimentally investigate springback. The third section gives a review of

constitutive models (anisotropic yield criteria and hardening laws) used to numerically simulate

sheet metal forming and springback. And the final section describes various experimental testing

facilities that researchers have developed to characterize the cyclic behaviour of sheet materials

in view of obtaining material input data for numerical simulations.

**2.1 SPRINGBACK IN STAMPED PARTS **

In the automotive industry, high strength steel sheets and low density sheet metals have

become a necessity in order to reduce the weight of the vehicle body-in-white. However, the

increased use of materials with high strength and/or low elastic modulus as well as reduced

gauges leads to a significant increase in the amount of springback in stamped parts. Therefore,

springback has become a major challenge in regards to manufacturing lightweight automotive

components.

During the stamping of a sheet metal component, the sheet material is often subject to

7

stress distribution in the part after forming, and especially the stress gradient through the

thickness, is responsible for the nature and magnitude of springback. For example, Fig. 2.1

shows the stress distribution in a sheet material at different stages throughout the process of

being formed into a cup and after the part is allowed to springback. The non-uniform distribution

of stress in the part is very evident at each stage.

Figure 2.1Springback simulation of sheet metal cup in stamping

Depending on the type of forming process, the shape of the as-formed part, the sheet

mechanical properties, the selection of industrial process parameters and the stress distribution in

the formed part, the shape distortions due to springback can manifest themselves in a variety of

ways [2]. Because springback is so part and process-dependent, it can be very difficult to control

the geometry and dimensional accuracy of stamped sheet metal components. For example,

springback can cause twisting of the entire part, stretched areas tend to shrink, bent or flanged

edges will unbend to some extent (Fig. 2.2a) and drawn channel sections can exhibit curling of

the sidewalls (Fig. 2.2b and Fig. 2.3). Researchers have defined six common classes of

springback as follows [2]:

**(a) **

**(c) **
**(b) **

**(e) **

8 1) Sidewall opening (Figure 2.2a)

2) Sidewall Curl (Figure 2.2b)

3) Edge line warping or bow (Figure 2.2c)

4) Twist

5) Global shape change

6) Surface distortion

Figure 2.2 Different types of springback (a) wall opening (b) wall curl (c) bow [2]

Figure 2.3 Sidewall curl in a drawn channel section [2]

In order to minimize the distortions due to springback, efforts have typically been made

on two fronts: *a*) adjustments can be made to critical process factors such as blank holding force,

die clearances, ram velocity, lubrication, drawbead restraining force, etc. [3], and *b*) springback

is numerically predicted and compensated for at the tool design stage [4, 5]. The first approach is

essentially a pragmatic way to minimize springback due to variations in the mechanical

9

properties of incoming sheets after the stamping dies have been built. This type of springback

correction tends to have a limited impact and is only used to make minor adjustments since the

stress distribution in the part is largely determined by the deformation history of the sheet metal

in the dies. Process changes are rarely sufficient to eliminate springback problems that result

from a poorly designed tool. The second approach endeavours to optimize the forming process

and the design of the dies before they are built, so that the flow of metal during the stamping

process can be as even and uniform as possible and any gradients in residual stresses can be

minimized. Nowadays, this is the most cost-effective approach to springback compensation.

**2.2 EXPERIMENTAL SPRINGBACK STUDIES AND SIMULATIVE TESTS **

The earliest experimental springback studies consist of simple bending tests. Ogawa et al.

[6] performed V-bending tests to predict the springback of the high strength steel sheets and

observed that springback drastically decreases with increasing bottoming force. Fu and Mo [7]

conducted air bending test on high strength steel sheets and measured the springback angle and

radius. The geometric model of the air bending of sheet metal specimen proposed by Fu and Mo

is shown in Fig. 2.4.

Figure 2.4 Geometrical model of air bending of sheet metal [7]

10

In Fig. 2.4, c is the tool gap, t is sheet metal thickness, w is the die opening, r is the punch

radius, R is the bending radius, b is punch width, e is the punch displacement, and the springback

arc segment is defined by the bending arc segment of sheet metal after removal from the punch.

It is important to mention that in air bending springback can lead to changes of bending radius,

bending arc segment, and bending angle. The difference between the bending radius of a sheet

after unloading (R), and the punch radius (r) is defined as springback quantity of the bending

radius (∆ρ=R-r). The springback angle (∆β=α-θ) is the difference between the unloaded bend

angle (α) and the bend angle before springback (θ).

In many stamping operations, it is common for the sheet metal to be deformed in a plane

strain mode as a result of combined bending and tension. For instance, when sheet metal is

drawn through a drawbead and over the die shoulder radius as a result of the punch action (Fig.

2.5), it becomes subject to bending under tension. In order to thoroughly understand the

springback behaviour of sheet materials that have been deformed in this way a number of

researchers [7, 8] have developed simulative tests that reproduce bending-under-tension

deformation modes, and then have attempted to model the springback behaviour that was

observed experimentally.

11

Sanchez [8] developed a drawbead simulation testing apparatus that can apply both

bending and tension to a sheet specimen using three pin rollers. During testing the sheet metals

are bent, un-bent and bent in the reverse direction in a three-cycle sequence. A schematic of

Sanchez’ experimental binder geometry and theoretical model is shown in Fig. 2.6. During his

experiments, Sanchez observed that springback decreased with increasing tension and became

negligible for tensile forces approaching the tensile strength of the material. He reported that if

the coulomb friction on the pins increases by about 0.01, it would result in noticeably greater

tension forces and smaller curvature after springback [8].

Figure 2.6 Schematic of Sanchez’ three pin roller set-up for cyclic bending of sheet metal[8]

Schilp et al. [9] investigated the effects of three different factors on the springback

response after stretch-bending tests: the stretching method, the stretching length and the

stretching direction. They showed that when the bending radius to the sheet thickness ratio (R/t)

increases, the springback gradually increases and reaches a maximum when the ratio is R/t = 10,

with a 45o bending angle. In order to investigate the stretching effect, Schilp et al. [9]compared

four processes: bending without stretching (WS), pre-stretching and bending (PB), pre-stretching

plus simultaneous stretching and bending (PSB), and simultaneous stretching and bending (SB).

They compared the springback factor maintained a fixed R/t and changed the bending angles of

12

process the amount of springback increases drastically. The springback remained regular values

regardless of bending angle in SB process. As, R/t increases and the bending angle becomes

smaller, the SB process produces less springback than other process. They concluded that,

simultaneous stretching and bending can reduce the springback, and the variation of stretching

length has no distinct effect in the simultaneous stretching and bending process.

Lim et al. [10] conducted an experimental study using a draw-bend test (Fig. 2.7) to

determine the time-dependent springback at room temperature of four AHSS sheets, (DP600,

DP800, DP980 and TRIP780), and three conventional steel sheets (AKDQ, DQSK and HSLA).

After drawing the test strips over the tool radius and unloading them, they measured the

springback angle at regular time intervals up to 6 months after the test; the instantaneous

springback angle was called the time-independent springback angle. When the springback angle

continued to increase over time, it would eventually reach a saturation value; the difference

between the saturated angle and the instantaneous angle was called the time-dependent

springback angle. It was observed that both AHSS and conventional steels showed a decrease in

the instantaneous springback angle with increasing back force and tool radius. In addition, AHSS

with higher yield stress showed larger instantaneous springback angles compared to conventional

steels [10]. All AHSS demonstrated angle changes during the 6 months after testing, but the

conventional steels did not. It was observed that for DP800, DP980 and TRIP780 steels the

maximum time-dependent angle was attained only 2 weeks after testing, but for DP600 steel, the

angle change saturated a long time after testing (Fig. 2.8). Lim et al. also observed that the

13

Figure 2.7 Schematic of the draw-bend test[10].R is the roller radius,Fb is the back force, and

Δθ is the springback angle

Figure 2.8 Time-dependent springback in (a) DP600 (b) DP980 (c) TRIP780 strips subject to bending under tension [10].R/t is the roller radius to sheet thickness ratio,Fb is the back force,

and δθ is the time-dependent springback angle

In order to understand the time-dependent springback of AHSS, Lim et al. investigated

two mechanisms: an elastic deformation and residual stress driven creep. They used a simple

finite element model based on residual stress-driven creep model to simulate their experiments,

but found that the model over-estimated the experimentally measured springback angles by a

factor of two.

14

Wagoner et al. [11, 12, 13, 14, 15, 16] carried out extensive research on springback

prediction using draw bend tests. In order to determine the springback effect, Wagoner et al. [11]

performed two-dimensional stretch draw bend tests adjusting three process parameters: tool

radius, friction and back force. They found that the applied back force dominated the springback

sensitivity that R/t had a modest effect and friction had a minor effect on springback. The

springback decreased with increasing R/t ratio and increasing back force. The springback can be

decreased up to about 90% and 25% by increasing the tensile stress and the R/t ratio,

respectively [12].

Wagoner et al. [14] devised draw-bend tests to measure and predict springback under

controlled conditions. They observed a discrepancy between the simulation and experimental

results. It might have been due to the use of the isotropic hardening model that does not

reproduce the Bauschinger effect. The springback angle is very sensitive to the hardening model.

In order to generate a mixed hardening law that could describe the active yield surface and

bounding surface, Wagoner et al. [15] devised a tension-compression-type model. They showed

that the springback angles were reduced by using a compression-tension or tension-compression

model instead of the isotropic hardening model. The modified nonlinear hardening model

developed by Wagoner et al. [16] showed that the predicted springback angle tends to linearly

decrease with an increasing back force. They concluded that accurate springback simulations

might obtained by a judicious combination of material properties, R/t, and sheet tension.

Carden et al. [17] conducted bending and un-bending tests to measure ‘sidewall curl’.

They reported that the curl is minimized for a variety of steels when R/t = 2, and smaller R/t

15

**2.3 PREDICTION OF SPRINGBACK **

As mentioned earlier, the most efficient way to build stamping dies that accurately

compensate for springback is to numerically simulate the forming operation and the subsequent

elastic unloading of the part. Such numerical simulations are generally performed with a finite

element code in which the sheet material behaviour is described by an appropriate constitutive

model. In the classical theory of plasticity, a constitutive model is comprised of a flow curve that

defines how the material hardens during plastic deformation, and a yield criterion and a

hardening model. The yield criterion is a function that represents the stress states at which the

material starts to yield, i.e. when the transition from elastic to plastic behaviour occurs, and these

stress states form a convex surface, called the yield surface. The hardening law describes how

the yield surface evolves in stress space as a function of plastic deformation. In this section, the

yield criteria and hardening rules that are most commonly used to simulate sheet metal forming

and springback will be presented.

2.3.1 PLASTICITY AND ANISOTROPIC YIELD FUNCTIONS

The two simplest yield criteria were proposed by Tresca [18 and von Mises [19 and

determine the onset of yielding of isotropic materials [20]. Since most sheet materials display

some level of anisotropy (through the thickness or in the plane), many researchers (Hill 1948,

1979, 1990, 1993, Hosford 1979, Barlat1989, Barlat1991, Barlat1994, Barlat1996, Barlat 2000,

Karafillis1993, Cazacu & Barlat 2003, Banabic & Balan 2003) have proposed plane-stress

anisotropic yield criteria to represent the behaviour of orthotropic sheet materials. Among all

these criteria, Hill’s (1948, 1990), and Barlat’s (1991, 2000) yield criteria are the most widely

16 Hill’s Yield Criteria

Hill [22] was the first to propose a yield criterion for anisotropic materials. Hill’s 1948

yield criterion is an extension of von Mises’ criterion for isotropic materials and describes the

yielding of anisotropic materials using additional material constants. Due to its mathematical

simplicity, Hill’s 1948 quadratic yield function continues to be widely used for metal forming

simulations of orthotropic steel sheets [23].One of Hill’s more recent yield criteria (1990) is also

used when additional precision is required, such as for the prediction of earing in drawn cups.

Barlat’s Yield Criteria

To properly describe the yield and anisotropy of aluminum alloys Barlat et al. [24,25]

proposed a plane-stress yield criterion in 1989 that has been successively modified in 1991,

1996, 2000, and 2003. These yield criteria are widely used for modelling the behaviour of FCC

materials such as, aluminum alloys [26]. Barlat’s Yield 2000 criterion also accurately predicts

the behaviour of sheet steels e.g. DP600, HSLA [27].

These various yield functions describe the initial stress states at which yielding begins but

do not account for the evolutionof material anisotropy during on-going plastic deformation [26].

A hardening law is required to model the evolution of the yield surface.

2.3.2 HARDENING LAWS

At a given material point the yield surface evolves in stress space as a result of work

hardening, and it is important to accurately describe the way in which it evolves because, in the

numerical simulation. The shape of the yield surface determines the direction of the plastic strain

17

The hardening law models the possible changes in shape, size and orientation of the yield surface

at each increment during the plastic deformation.

As was pointed out earlier, cyclic loading is a very common type of loading in sheet

metal forming processes. Since reverse loading can lead not only to elastic unloading but also to

plastic deformation in a reverse direction, the hardening rule should be able to accurately predict

the hardening behaviour for cyclic loading. Over the past few decades, researchers have

developed several hardening models and the most important ones will be described below.

Isotropic Hardening

When the expansion of the yield surface is uniform in all directions in stress space, the

hardening is referred to as isotropic [28]. Indeed, many materials can be considered isotropic in

the annealed state, and the Bauschinger effect and the anisotropy developed due to deformation

may be neglected [29]. This hardening law has been widely adopted in the industry since it is

easy to implement (i.e. it does not require any cyclic testing to be carried out), although it may

give large errors under reverse loading [30]. The yield function equation for isotropic hardening

is written as:

𝑓 ( , 𝑝) = − 𝑦 (𝑝) =0 2.1

where is the effective stress, 𝑝 is the accumulated effective plastic strain, and 𝑦 (𝑝) is the

yield stress which might be of the form :

𝑦𝑝 = 𝑦0 + *r* (𝑝) 2.2

where 𝑦0 is the initial yield stresses and 𝑟(𝑝) is called the isotropic hardening function.

Fig. 2.9 schematically shows the relationship between the uniaxial stress-strain curve and the

18

yield surface, the yield stress in the reverse loading is equal to that in forward loading. Therefore

isotropic hardening is not able to describe the Bauschinger effect which is often observed under

reverse loading.

Figure 2.9 Isotropic hardening of the yield surface with plastic deformation, and the corresponding uniaxial stress-strain curve [28]

Kinematic Hardening

Kinematic hardening was developed to model the work hardening behaviour of materials

that exhibit the Bauschinger effect (a decrease in the yield stress in compression as a result of

previous loading in tension). Kinematic hardening assumes that the yield surface merely

translates in stress space during plastic deformation (Fig. 2.10), and the translation in one

direction results in a reduction of the yield stress in the opposite direction [31]. Therefore, the

shape and size of the subsequent yield surface do not change during plastic deformation. Fig.

19

Figure 2.10 Kinematic hardening showing (a) the transitions, | | of the yielding surface with plastic strain, and (b) the resulting stress-strain curve with shifted yield stress in compression-the

Bauschinger effect [28]

With continued loading, the material deforms plastically and the yield surface translates.

When load point (1) is achieved the load is reversed, so that the material deforms elastically until

point (2) is reached, when the load point is again in contact with the yield surface. Therefore, the

elastic region is much smaller than that predicted with isotropic hardening. In the case of

kinematic hardening, the equation of the yield surface is written as:

𝑓 ( – α) − 𝑦 = 0 2.3

where α is called the back stress tensor which determines the location of the centre of the yield

surface.

Prager [32] and Ziegler [31] were the first to develop kinematic hardening rules.

However, the classical kinematic hardening model tends to over-predict the Bauschinger effect,

20

loading, such as the smooth transient re-yielding behaviour, work hardening stagnation or the

creep (ratchetting) effect under cyclic stress [33].

Non-Linear Kinematic Hardening

Armstrong and Frederick [34] developed a nonlinear kinematic hardening (NKH) model

by modifying the linear hardening law proposed by Prager [32]. Chaboche [35] also predicted

the smooth transient behaviour by introducing an additional nonlinear back-stress term to

Prager’s linear kinematic hardening model which could not account for the permanent softening

behaviour during the reverse loading. Li [36] developed a pure nonlinear kinematic approach

with finite element implementation to perform a shakedown analysis of materials. The

experimental and simulated cyclic behaviour of a DP600 sheet steel is shown in Fig. 2.11

developed by Taherizadeh et al. [2, 37] using a NHK hardening model.

21

Yoshida et al. [38] identified the material parameters for the NKH model using an

iterative multipoint approximation of the data obtained from uniform bending tests. Chun et al.

[39, 40] and Vladimirov et al. [41] used NKH to determine the anisotropic parameter of sheet

metals. Brunet et al.[42] extended the NKH to the plastic anisotropy and identified the material

constants based on four point bending experiments and a Sequential Quadratic Programming

algorithm.

Mixed Hardening

Many researchers now use a combined isotropic-kinematic hardening (mixed hardening)

model in order to take advantage of both models and more accurately predict the cyclic

behaviour of certain sheet materials. For instance, Yoshida and Uemori [43], Geng et al. [44],

Chaboche [35], Chaboche and Rousselier [45], Khan and Jackson [46] used the mixed hardening

model, since it can reproduce the Bauschinger effect, the smooth elastic-plastic transition upon

re-yielding and the isotropic hardening effect. A schematic of the mixed hardening model is

shown in Fig. 2.12.

In order to improve the prediction capability of reverse loading and springback

behaviour, a modified Chaboche-type combined isotropic-kinematic hardening model was

developed by Chung et al. [47] and Lee et al. [48] to effectively describe the Bauschinger effect

and the transient behaviour. However, Kim et al. [49] reported that the modified Chaboche

model cannot account for the permanent softening behaviour during the reverse loading. Chow et

al. [50] proposed a generalized mixed isotropic kinematic hardening plasticity model coupled

22

Figure 2.12 Schematic illustrations of combined kinematic and isotropic hardening [28]

Taejoon et al. [51] analyzed the time dependent springback behaviour of a 6022-T4

aluminum alloy sheet using a visco-elastic/plastic constitutive law. They also used the combined

isotropic-kinematic hardening law to represent the Bauschinger behaviour and transient

hardening, and the non-quadratic anisotropic yield function Yld2000-2D was applied to account

for anisotropic yield behaviour. Using the results of draw bend tests, they showed that this

constitutive law and formulation are valid for time dependent springback.

Taherizadeh et al. [23] developed a non-associated flow rule (NAFR) with mixed

hardening. They showed that the non-associated mixed hardening model significantly improved

the prediction of springback in the sidewall of drawn channel sections and the prediction of

earing in the cup drawing process. Taherizadeh et al. [37] also suggested that the mixed

23

al. [52] proposed a combined isotropic and kinematic hardening model and used an inverse

approach to identify parameters using the monotonic tensile and cyclic experimental indentation

curves.

A Rotational-Isotropic-Kinematic (RIK) hardening model was developed by Choi [53] to

transform the major effects of micro-mechanical deformation behaviours to a phenomenological

model. The proposed RIK model allows the yield surface to grow (isotropic), to translate

(kinematic) and even to rotate (rotational) as the deformation progresses. The RIK model was

formulated based on the Armstrong-Frederick type kinematic hardening model and on the

rotation of the symmetry axes of anisotropy with the plastic spin theory. The ability of the model

was demonstrated by the multi-path loading of ‘tension-shear’ and ‘reverse-shear’ to reveal the

‘crossing’ and ‘Bauschinger’ effects [53].

Multi-surface Hardening Models

The use of multiple-surface models instead of the single yield surface is an alternate way

to describe the permanent softening and non-symmetric reloading behaviours. Dafalias and

Popov [54] analyzed two-surface kinematic hardening models through complex loading that was

developed by Krieg [55]. Yoshida and Uemori (YU) [43] proposed a two-surface plasticity

model that assumes kinematic hardening of the yield surface within a bounding surface that

expands isotropically and their two-surface model is capable of reproducing the transient

Bauschinger effect, permanent softening and work hardening stagnation in large elasto-plastic

deformation. The YU two-surface model is schematically shown in Fig. 2.13. The inner surface,

or yield surface, determines the elastic domain of the material in stress space and translates in

24

Figure 2.13 Schematic illustration of Yoshida-Uemori two-surface model [43]

In Fig. 2.13, Dp is the rate of plastic deformation, np is the unit vector direction of plastic

strain rate, S is the Cauchy stress deviator, αb is the back stress deviator, Y is the radius of the

yield surface in deviatoric stress space, β is the center of the bounding surface, B is the initial

size, R is the isotropic hardening component, is the relative kinematic motion of the yield

surface with respect to the bounding surface and is the unit vector direction of relative

kinematic motion. Fig.2.14 shows how these particular material responses appear on a

25

Figure 2.14 Schematic illustration of the stress-strain behaviour of certain materials [56]

McDowell [57] and Lee et al. [58] defined two independent hardening parameters for the

kinematic evolution of the yield and bounding surfaces in the YU model. Cardoso and Yoon [59]

proposed another two-surface kinematic hardening model. Hashiguchi [61] used a three-surface

model; Hassan et al. [61, 62], and Mroz [63] used a model with multiple yield surfaces to

describe the cyclic loading. Multi-surface models are capable of describing the Bauschinger

effect and the nonlinear transient behaviour, but require a large number of yield surfaces to

obtain the smooth transient behaviour.

2.3.3 NUMERICAL SIMULATION OF SPRINGBACK

The complexity of predicting springback in stamped components is such that many

researchers around the world have been working for the last few decades to develop numerical

tools and methodologies that enable them to predict springback in a rigorous and reliable

manner. As was discussed in the previous section, the selection of a constitutive model that is

26

However, the accuracy of simulation results depends on many other parameters, such as the

numerical implementation of the constitutive model into a finite element program, the accuracy

of the forming simulation with its specific challenges of modeling contact and friction, as well as

the selection of a host of numerical parameters. In this section, the work of various researchers

will be presented with a view to highlighting the most important aspects of numerical simulation

of springback.

Hußnatter and Merklein [64], Thuillier et al. [65], Lee et al. [48] and Oliveira et al. [66]

reported that springback prediction strongly depends on the accurate simulation and realistic

modeling of the forming operation. To predict springback, Thuillier et al. and Oliveira et al. [65,

66] emphasized that the accuracy of the stress state at the end of the forming simulation is

critical to the accurate prediction of springback. They mentioned that constitutive models should

have a reliable description of the material behaviour, especially in terms of anisotropy and work

hardening during loading and unloading.

Cao [67] reported that springback is connected with several factors such as, tool

structure, sheet material properties, sheet material geometries, friction etc. The relationships

among those factors are complex and non-linear. Therefore, it is difficult to find a mathematical

model that can predict the springback perfectly.

Verma et al. [68] reported that the accuracy of springback prediction depends on the yield

surface shape, the number of integration points, the type of element used in numerical

simulations, the incorporation of permanent softening, and the strain-dependent elastic modulus.

Moreover, it is difficult to conclude with certainty the reasons for inaccuracies since the effects

27

Oliveira et al. [66] used several constitutive work hardening models such as classical

isotropic, non linear kinematic and Teodosiu’s micro structural model in order to predict the

springback of DP600 and mild steel (DC06). They used Swift’s power law to describe the

classical isotropic work-hardening, the Lemaitre and Chaboche law [69] to describe the

non-linear kinematic hardening model and Teodosiu’s micro structural work-hardening model.

However, the effect of drawbead penetration was not studied in their work.

Many researchers such as, Hußnatter and Merklein [64], Lee et al. [48], Banu et al.[70],

Oliveira et al.[66], Vladimirov et al.[71], and Yoshida[72] have shown that the Bauschinger

effect (straining in one direction reduces the yield stress in the opposite direction) has a strong

influence on the prediction of springback. Zhang and Hu [73] calculated the springback by using

three different cyclic material models such as, isotropic, kinematic and directional hardening,

and observed a remarkable difference in results. Campana et al. [74] used a combined

isotropic-kinematic hardening model to predict the forming and springback behaviour of various AHSS

sheets.

Arwidson [75] reported that when the sheet material was subjected to cyclic loading

conditions springback prediction must consider the Bauschinger effect. He showed that the

prediction of springback depends on the accuracy of reproducing both the Bauschinger effect and

plastic shakedown using a combined isotropic/non-linear kinematic hardening (NKH) material

model. He concluded that applying tension drastically reduced springback and the friction in the

normal range encountered in sheet metal forming had little effect on springback [75].

Chun et al. [76, 77] used finite element simulations associated with an anisotropic non

28

drawing in the presence of draw beads. However, their drawbead model predicted an excessively

large compressive stress at the surface of the sheet at the level of the exit bead.

Taherizadeh et al. [78] showed that the springback results are significantly dependent on

the type of hardening model when one compares between pure isotropic hardening (IH) and

combined isotropic-nonlinear kinematic hardening. They also reported that the prediction of

springback is more sensitive to the hardening model than to the yield function[37]. Taherizadeh

et al. [2] conducted further studies to see the effect of drawbead penetration and restraining force

on the prediction of springback (Fig. 2.15). Comparing simulation results with experimental

springback data obtained from straight channel sections drawn in plane strain they showed that

the IH model generally overestimates the amount of springback due to the high stresses derived

by this model. On the other hand, the NKH model was able to predict the springback

significantly more accurately than the IH model. In this work, the channel sidewall profiles

predicted by all models were somewhat different from the experimental springback data because

the hardening parameters used in the hardening model were identified from the cyclic

tension-compression tests in which the amount of reverse strain was fairly small compared to the amount

of plastic strain that the sheet metal underwent during channel forming. These authors

recommended that a large reverse strain in the cyclic characterization test would enable more